Sensing low concentrations of CO using ﬂame-spray-made Pt/SnO2
L. Ma¨dler1,4,*, T. Sahm2, A. Gurlo2, J.-D. Grunwaldt3, N. Barsan2, U. Weimar2and S.E. Pratsinis1 1
Particle Technology Laboratory, Swiss Federal Institute of Technology (ETH) Zurich, Sonneggstrasse 3, CH-8092, Zu¨rich, Switzerland;2Institute of Physical and Theoretical Chemistry, University of Tu¨bingen, Auf der Morgenstelle 8, D-72076, Tu¨bingen, Germany;3Department of Chemistry and Applied Biosciences, Swiss Federal Institute of Technology (ETH) Zurich, Ho¨nggerberg, CH-8093, Zu¨rich, Switzerland;4Department of Chemical Engineering, University of California, Los Angeles, 5531-G Boelter Hall, Los Angeles, CA, 90095, USA; *Author for correspondence (Tel.: +310-825-9926; Fax: +310-206-4107; E-mail: firstname.lastname@example.org)
Received 6 April 2005; accepted in revised form 29 July 2005
Key words: gas sensor, CO detection, ﬂame spray pyrolysis, tin dioxide nanoparticles, platinum func-tionalization, XPS/EXAFS, combustion
Tin dioxide nanoparticles of diﬀerent sizes and platinum doping contents were synthesized in one step using the ﬂame spray pyrolysis (FSP) technique. The particles were used to fabricate semiconducting gas sensors for low level CO detection, i.e. with a CO gas concentration as low as 5 ppm in the absence and presence of water. Post treatment of the SnO2nanoparticles was not needed enabling the investigation of the metal oxide particle size eﬀect. Gas sensors based on tin dioxide with a primary particle size of 10 nm showed signals one order of magnitude higher than the ones corresponding to the primary particle size of 330 nm. In situplatinum functionalization of the SnO2during FSP synthesis resulted in higher sensor responses for the 0.2 wt% Pt-content than for the 2.0 wt% Pt. The eﬀect is mainly attributed to catalytic consumption of CO and to the associated reduced sensor response. Pure and functionalized tin dioxide nanoparticles have been characterized by Brunauer, Emmett and Teller (BET) surface area determination, X-ray diﬀraction (XRD), high resolution transmission electron microscopy (HRTEM) and scanning transmission electron microscopy (STEM) while the platinum oxidation state and dispersion have been investigated by X-ray photoelectron spectroscopy (XPS) and extended X-ray absorption ﬁne structure (EXAFS). The sensors showed high stability (up to 20 days) and are suitable for low level CO detection: <10 ppm according to European and 50 ppm according to US legislation, respectively.
Gas sensors based on semiconducting metal oxides are one of the most investigated group of gas sen-sors (Pearce et al., 2004). For them, the
conduc-tanceGor electrical resistance R is monitored as a
function of the concentration of target gases and subjected to further data treatment and processing.
SnO2-based sensors are the best-understood
prototype of oxide-based gas sensors and, in par-ticular, have been used widely in gas sensing under atmospheric conditions (Barsan et al.,1999;
Bar-san & Weimar2003; Eranna et al., 2004).
One of today’s challenges in carbon monoxide (CO) monitoring is the low concentration range (i.e. below 50 ppm) because of the fact that it is a toxic
gas accompanying nearly all combustion processes. The US Occupational Safety and Health Adminis-tration (OSHA) has set a general industry Permis-sible Exposure Level (PEL) for CO of 50 ppm averaged over an 8 h work shift (
http://www.osh-a.com). The American Conference of
Governmen-tal Industrial Hygienists (ACGIH), a private professional organization, has adopted a threshold limit value (TLV) of 25 ppm. In Europe, the limit value of CO (maximum daily 8 h mean) for the protection of human health to be met in 2005 is set at 10 mg/m3(8.75 ppm) (EN, 2000). At present,
for example, in Germany, there are two kinds of occupational exposure limits (OELs) for air in the workplace: Technische Richtkonzentrationen (TRKs), which are technical guidance concentra-tions, and Maximale Arbeitsplatz Konzentrationen (MAKs), which give the maximum concentration of a chemical substance in the workplace (the MAK-values are daily 8 h time-weighed average values and apply to healthy adults). In Germany the MAK value for CO is set at 30 ppm.
For CO detection on metal-oxide (i.e. SnO2)
based gas sensors, it is well known and generally accepted that the CO reacts with the adsorbed oxygen ions (like O
2 or O)) getting oxidized to
CO2and the released electrons (sensing step) can
therefore return to the conduction band (CB) according to the scheme:
COðgasÞþ OðsÞ! CO2ðgasÞþ e (CB)
Water has a similar reaction path way with the absorbed oxygen radical and therefore the eﬀect of CO is often shielded by water (Sahm et al.,2005). To
enhance the sensing properties, SnO2is often
func-tionalized with diﬀerent noble metals (i.e. usually Pd, Pt, Au). In general, this decreases the response and recovery times, and increases the sensitivity, selec-tivity, reproducibility and stability of the sensors (Yamazoe, 1991; Sweizer-Berberich et al., 1996).
However, in each particular case – depending on the amount, chemical state, aggregation and localization of the atoms – the noble metal can inﬂuence the sensing properties in completely diﬀerent manner; no generalization can be made even for the same base material (i.e. SnO2) (Matsushima et al., 1988;
Yam-azoe,1991; Gaidi et al., 1998; Kappler et al., 1998;
Matko et al.,1999, 2002; Cabot et al., 2000, 2001,
2002; Dieguez et al., 2000). Usually, surface
func-tionalization leads to an improvement of the sensing
properties, while the doping with higher concentrations results in materials with poorer sensing properties (Grandjean et al.,2004).
More-over, the situation will be diﬀerent if the noble metal forms isolated metallic nanoparticles of a few na-nometers (‘‘metallic clusters’’) or is getting oxidized and diﬀusing into the lattice of base material (SnO2)
forming solid-solutions (this is especially favorable for platinum because PtO2has the crystalline
struc-ture of rutile – the same as cassiterite strucstruc-ture of SnO2).
The production of homogenous SnO2
nanopar-ticles by ﬂame spray pyrolysis (FSP) for gas sens-ing has been demonstrated successfully for senssens-ing of NO2and propanal (Sahm et al., 2004). In
gen-eral, FSP has the ability to control particle size, produce highly single crystalline nanoparticles (Ma¨dler et al., 2002a), and functionalize metal
oxides within on step, often called in situ, with
noble metals (Ma¨dler et al., 2003; Strobel et al.,
2003). Therefore, FSP is well suited to address the
eﬀects of tin dioxide nanoparticle properties such as size, crystallinity and platinum functionaliza-tion with regard to gas sensing performance and in particular CO detection. The resulting high exter-nal surface area, high noble metal dispersion and the absence of a powder post-calcinations step are further advantages of the FSP with regard to sensor manufacture.
An aerosol reactor was used to produce SnO2and
Pt/SnO2 nanoparticles by FSP (Ma¨dler et al.,
2002b). The liquid precursor was prepared by
diluting tin(II) 2-ethylhexanoic acid (Sigma-Aldrich, purity >98%) in toluene (Fluka, purity >99.5%) to obtain a 0.5 M precursor solution. For Pt/SnO2 synthesis, appropriate amounts of
platinum acetylacetonate (Pt(acac)2, Strem, purity
>98%) were added to the solution to obtain a platinum loading of 0.0, 0.2 and 2.0 wt%, respectively. The liquid precursor was fed by a syringe pump (Inotech R232) with a constant feed rate of 5 and 8 ml/min through a capillary of an outside-mixing two-phase nozzle. The liquid was dispersed into ﬁne droplets with 3 and 5 l/min oxygen (Pan Gas, 99.95%) maintaining a pressure
drop of 1.5 bar at the nozzle exit. All gas ﬂow rates were controlled by calibrated mass ﬂow controllers (Bronkhorst). In particular, the ﬂame spray was operated at two diﬀerent sets of ﬂow rates: 5 ml/ min liquid precursor feed rate with 5 l/min oxygen dispersion gas (deﬁned as 5/5) and 8 ml/min liquid precursor feed rate with 3 l/min oxygen dispersion gas (deﬁned as 8/3). The liquid spray was ignited by a premixed methane/oxygen (1.5 l/min/3.2 l/ min, respectively) ﬂame ring surrounding the nozzle exit (Ma¨dler et al.,2002b). A sintered metal
plate ring (8 mm wide, at inner radius of 9 mm from the center of nozzle) issued additional 5 l/min of oxygen as a shield gas. The powder was col-lected with the aid of a vacuum pump on a glass ﬁber ﬁlter (GF/D Whatman, 257 mm in diameter). During the experiment, the ﬁlter was placed in a water-cooled holder, 400 mm above the nozzle, keeping the oﬀ-gas temperature below 200°C. Powder characterization
X-ray diﬀraction patterns were recorded with Bruker AXS D8 Advance (40 kV, 40 mA) and used to obtain the crystallite size (dXRD) based on
the fundamental parameter approach and the Rietveld method (Cheary & Coelho,1998) with the
structural parameters of cassiterite (ICSD Coll. Code: 084576; Bolzan et al., 1997). A linear
background was used when matching the XRD patterns while microstrain was not considered. The BET powder speciﬁc surface area (SSA), was measured by nitrogen adsorption at 77 K (Mi-cromeritics Gemini 2375) after degassing the sample, at least, for 1 h at 150°C in nitrogen. Assuming monodisperse spherical primary parti-cles within an aggregate, the equivalent average primary particle diameter dBET was calculated by dBET=6/(SSA qp), where qpis the density of SnO2
(6.85 g/cm3). Transmission electron microscopy
analysis was carried out with a Phillips CM30ST microscope (LaB6 cathode, 300 kV). Scanning
transmission electron microscopy (STEM) images were obtained with a high-angle annular dark-ﬁeld (HAADF) detector (Zcontrast).
X-ray photoelectron spectroscopy (XPS) mea-surements were performed on a Leybold Heraeus LHS11 MCD instrument using MgKa (1253.6 eV) radiation (Grunwaldt et al., 1997). The analyzer
was operated at 150 eV pass energy. The sample was ﬁxed on a sample holder on top of a graphite
foil and transferred to a load lock chamber where it was evacuated at room temperature for 2 h down to 10)6mbar. Finally, it was transferred to the
analysis chamber at a typical pressure of 10)9mbar. For quantiﬁcation of the composition
the following peaks were used: O1s, C1s, Pt4f (both Pt4f5/2and Pt4f7/2), and Sn3d5/2. The Shirley-type
background subtraction and quantiﬁcation of the surface concentration were performed using the SPECSLAB software package (SPECSLAB, Pro-gram software for XPS, ISS, and UPS, Specs., Berlin, Germany). Sensitivity factors used for cal-culation of the surface composition were taken from the SPECSLAB program (SPECSLAB, Pro-gram software for XPS, ISS, and UPS, Specs., Berlin, Germany). The spectra were not corrected for the shift since only for the SnO2sample partial
charging was observed. The 2.0 wt% Pt/SnO2
sample was not charged at all, while the 0.2 wt% Pt/SnO2sample showed a small fraction (ca. 5%)
that was charged. Note that the Pt to Sn surface ratio was determined by acquiring separate spectra over about 24 h in case of 0.2 wt% Pt/SnO2 to
obtain a suﬃcient signal-to-noise ratio.
In order to gain further insight into the structure of the Pt dopants, additionally, EXAFS spectra at the Pt L3-edge were taken of as-prepared powder
0.2 wt% Pt/SnO2 and 2.0 wt% Pt/SnO2 samples.
Note that the low loading of Pt on a strongly X-ray absorbing support requires detection in the ﬂuorescence mode (Iwasawa,1996; Kappen et al.,
2002). This was achieved with a 5-element solid
state detector (Canberra) at ANKA-XAS in Kar-lsruhe (Forschungszentrum KarKar-lsruhe, Germany). The as-prepared samples were monitored after pressing them to self supporting discs/pellets. Data were collected between 11.45 and 12.3 keV in the step-scanning mode using a Si(111) double crystal for monochromatization of the X-rays (typically detuned to 60% of the intensity to remove higher harmonics). The raw data were energy-calibrated with the Pt metal foil (Pt L3-edge), background
corrected, and normalized using the WINXAS 3.1 program package (Ressler, 1998). Fourier
trans-formation was applied in the range 2.5–12 A˚)1.
DC electrical measurements (sensor tests) have been performed to monitor the response to CO in syn-thetic air with 0% (dry), 10% and 50% relative
humidity (r.h.) at 20°C. The sensing layers were fabricated by classical thick ﬁlm deposition tech-nology (i.e. screen printing or drop-coating, see Sahm et al.,submitted) of a suspension of the
FSP-made nanoparticles on the alumina substrates with interdigitated Pt electrodes on the front side and a heater on the back side (Barsan & Weimar,2003).
For the comparison tests, commercially available SnO2 powder (Sigma-Aldrich, mesh 325, d330 nm) was also used. After the deposition of
the sensing layer, the as-obtained sensors were ﬁred in air in a moving belt oven (Centrotherm Centronic DO 1600-60-D5) with four individually operated heating zones. The velocity of the moving belt was adjusted to allow the sensors to stay in the maximum temperature zone (actually, at 500°C) for 10 min.
The conventional sensor tests were performed with a set of four sensors placed in a teﬂon-made test chamber and operated in the same conditions. The operating temperature of the sensors was adjusted between 200 and 400°C for individual sensor tests. A computer driven gas-mixing system provided the analyte gas for sensing evaluation (Kappler, 2001). CO catalytic conversion
mea-surements have been performed for 0.2 and 2.0 wt% Pt doped sensors by the use of eight identical sensors, respectively. These sensors have been placed into two test-chambers that were connected in series. The ﬁrst one contained a single sensor, whereas in the second one seven sensors were arranged along the gas ﬂow with always two sensors opposing each other. For stability tests, a set of four sensors (two sensors with 0 wt% Pt and two with 0.2 wt% Pt) has been exposed to a test cycle of three diﬀerent CO concentrations (10, 240 and 50 ppm) repeating every second day for a period of 20 days. The sensing properties were assessed through sensor signal S, reported as the
resistance ratio Rair/Rgas, where Rgas and Rair
denote the sensors’ resistances in the presence and absence of CO, respectively (please note that the sensor signal has units of ohm/ohm).
Results and discussion
Eﬀect of nanoparticle size on sensing properties Characterization of tin dioxide nanoparticles Pure SnO2 nanoparticles were produced at two
conditions: ﬂame 5/5 or 8/3. These conditions
correspond to relatively low temperatures and dilute aerosols or high temperatures and dense aerosols, respectively (Ma¨dler & Pratsinis, 2002).
In general, increasing the ratio of the precursor liquid to dispersion gas ﬂow rate increased the average primary particle size as determined by BET from about 9.9 (88.1 m2/g) to 19.4 nm
(45.2 m2/g). Figure 1 shows the corresponding
X-ray diﬀraction patterns of these powders which were present in the cassiterite phase of tin dioxide. Applying fundamental parameter and Rietveld analysis on SnO2 (Sahm et al., 2004) resulted in
average crystallite sizes of 10.7 and 19.8 nm for the particles made with ﬂames 5/5 and 8/3, respec-tively. The excellent agreement between the corre-sponding BET and XRD average size of the powders indicates the presence of monocrystalline particles. The high crystallinity and the presence of single crystalline primary particles was conﬁrmed by the high resolution transmission electron anal-ysis and the corresponding electron diﬀraction pattern of a powder produced with the 5/5 con-ﬁguration (ﬁgure2). Furthermore, the average size
of the individual primary particles in the HRTEM image is in good qualitative agreement with the reported dBET and dXRD. The precise control of
Figure 1. X-ray diﬀraction patterns of pure SnO2powders
made at diﬀerent ﬂame conditions. Increasing the precursor to oxygen feed ratio increases the tin dioxide grain size and therefore narrows the peak width. Excellent agreement be-tween XRD and BET analysis indicates the presence of monocrystalline SnO2 particles. Numbers in brackets
particle size and the high crystallinity of the FSP products have been demonstrated previously for various single oxide powders such as silica, ceria, bismuth oxide and zinc oxide (Ma¨dler et al.,2002a,
b; Ma¨dler & Pratsinis, 2002; Tani et al., 2002).
Characterization of sensors made from pure tin dioxide
For benchmarking reason, sensors based on sens-ing materials obtained by FSP were compared to sensors based on commercially available tin diox-ide (Figure3). For the case of a commercial
powder from Sigma-Aldrich, with an average diameter of 330 nm, one records two orders of magnitude lower total resistance; this might be an advantage in practical applications because of the possibility of using simple read out electronics. However, the sensor signal (at 500 ppm; this high CO concentration was chosen due to the low sensitivity of sensors based on commercial SnO2
powder) is drastically increased for the FSP materials with primary particle size 10 nm (where it reaches a maximum). The reasons for the increase, corresponding to the lowest grain size value, could be: the higher speciﬁc surface area within the sensing layer, the larger inﬂuence of the surface phenomena (the relative increase of depletion layer in comparison with the particle size itself), a diﬀerent surface microstructure that induces a diﬀerent reactivity, a diﬀerent concen-tration of bulk defects that results in a diﬀerent availability of free charge carriers, etc.
A detailed study of the grain size eﬀects on sensors with reasonable good sensor response is
limited at the moment; the fabrication of particles smaller than 10 nm is possible by FSP but their processing into sensing layers by conventional ﬁlm deposition techniques (here screen printing) is very diﬃcult. In general, the eﬀect of grain size on sensing performance is still under debate since the work and models of Xu et al. (1991) and
Roths-child and Komem(2004). It is diﬃcult to compare
results and estimate the inﬂuence of the particle size on gas sensing properties because other parameters which inﬂuence the electrical properties
Figure 2. High resolution TEM and the electron diﬀraction pattern of particles produced in the ﬂame 5/5. The tin dioxide powder shows high crystallinity and individual particles are mostly monocrystalline.
Figure 3. Resistance (left axis, open symbols) and sensor signal (right axis, ﬁlled squares) for pure SnO2sensors of
diﬀerent particle sizes. With increasing particle diameter the resistance in air (s), in 500 ppm CO (h) and in 1000 ppm CO (n) decreases. Also the sensor signal for 500 ppm CO (n) decreases with increasing particle size. The measure-ments have been performed on drop-coated sensors at 350°C (ﬂame 8/3 and commercial powders) and screen-printed sensors at 400°C (ﬂame 5/5 powder) in dry air.
of SnO2gas sensor were not reported in most of
the previous experiments. The change in grain size was for example accompanied by variations in other microstructural features; therefore the con-clusion about size dependence of gas sensitivity could be misleading.
As the highest sensor signals came from the smallest tin dioxide grain size (ﬂame 5/5) these particles were investigated in detail. Figure4
pre-sents the sensor response when tested at very low CO concentrations in the range from 5 to 50 ppm at diﬀerent operating temperatures. In general, the sensor shows high signal values and its perfor-mance is best at an operating temperature of 300°C.
Eﬀect of SnO2nanoparticle functionalization
Characterization of platinum doping
Platinum doping of tin dioxide is performedin situ
with the FSP process by dissolving the corre-sponding components in the liquid precursor/fuel. The ﬁrstin situ functionalization of metal oxides
with platinum in a ﬂame process was demon-strated by Johannessen and Koutsopoulos (2002)
while the highly eﬃcient platinum doping by the FSP process was outlined for a Pt/Al2O3catalyst
by Strobel et al. (2003). In their study it was
additionally demonstrated that platinum is present as highly dispersed clusters and the nominal mass loading is preserved in the ﬁnal product.
Figure5 shows a scanning transmission electron
microscopy (STEM) image in Z-contrast of tin dioxide with a 2.0 wt% platinum doping made with at the ﬂame 5/5. The inherent Z-contrast diﬀerence between tin and platinum is not very high, resulting in a rather blurred image. However, the picture reveals clearly the absence of particle inhomogeneities and proofs the presence of the platinum by the corresponding EDX analysis of
Figure 4. Temperature dependence of the sensor signal of pure SnO2sensors for diﬀerent CO concentrations in dry
air. A power law dependence has been observed for all examined temperatures.
Figure 5. Left: Scanning transmission electron microscopy (STEM) image in Z-contrast of tin dioxide with a 2.0 wt% plat-inum doping (ﬂame 5/5) indicating the absence of particle inhomogeneities. Right: Corresponding EDX analysis. The presence of the copper and carbon signals in the EDX spectrum resulted from the carbon coated copper TEM grid used.
that section (Figure4). The presence of the copper
and carbon signals in the EDX spectrum resulted from the carbon coated copper TEM grid used.
Figure6 shows the tin dioxide XRD patterns
for diﬀerent platinum loadings of 0.0, 0.2 and 2.0 wt% (ﬂame 5/5). The highly crystalline cassit-erite structure and the tin dioxide crystallite size were not inﬂuenced by the addition of platinum resulting in an unchanged BET surface area. The employed small platinum loadings at these FSP conditions could not be detected by XRD indi-cating the absence of large (10 nm and larger) crystalline platinum particles. Detailed informa-tion about the platinum can only be obtained from surface sensitive or element-speciﬁc analysis methods. The XPS analysis resulted in a theoreti-cal Pt/Sn ratio of 0.016:1 in 2.0 wt% Pt/SnO2
which is somewhat lower than the observed 0.006:1 ratio but may be explained with incorpo-ration of Pt into the SnO2-lattice (Table1). Note
also that the relative surface composition is more straightforward to interpret than the absolute surface composition. The relative Pt/Sn ratio evi-dences that the 0.2 wt% Pt/SnO2sample is better
dispersed (Table1). Interestingly, both platinum
doped samples show hardly any charging in XPS, while the SnO2sample does (Table 1).
The binding energies observed for tin dioxide are typical for those reported for SnIV
(Muilen-berg,1979). The analysis of the Pt 4f peaks shows
only one dominant species which is signiﬁcantly higher in binding energy than that reported for Pt0. It has been reported that Pt foil has Pt 4f7/2
and Pt 4f5/2 peaks at 70.7–70.9 and 74.0–
74.15 eV, respectively (Kim et al., 1971;
Muilen-berg,1979; Yang et al., 1997). The Pt 4f5/2peaks
of Pt2+and Pt4+species are located around 72.5
and 73.5–74.0 eV, respectively (Kappler et al., 1998; Muilenberg, 1979). The Pt 4f peaks
observed in the two Pt-doped SnO2 samples are
closely related to Pt2+-species. However, the
slight shift to lower binding energies may indicate some reduced species or loss of oxygen. No PtO2
species as in Dieguez et al. (2000) were detected.
Only one dominant species was found and a partially reduced Pt-species may be correlated to the semiconducting properties of SnO2(note also
that charging was observed). Furthermore, pumping in ultrahigh vacuum may result in a partial reduction of the platinum, leading to smaller shifts than expected for Pt2+. Therefore,
EXAFS spectra were recorded under ambient conditions without evacuation (see results further below).
At normal conditions under air, Pt is in oxidized state as revealed both by ﬂ-XANES (X-ray Absorption Near Edge Structure in the ﬂuores-cence mode) and by ﬂ-EXAFS (Figure7) for the
sensors made from FSP nanoparticles. The strong whiteline in XANES indicates that the Pt-species are well oxidized in the SnO2lattice (Gaidi et al.,
1998, 2000; Bazin et al., 1999; Kappen et al.,
2002). Hence, these results show that already
under vacuum or during X-ray irradiation in the XPS chamber loss of oxygen occurs leading to slightly shifted Pt 4f-peaks in XPS. Also the Fourier-transformed EXAFS data (Figure7b)
show that platinum is in oxidized state in ambient air. Further, both XANES and EXAFS indicate a high dispersion of the Pt inside the support since Pt is strongly oxidized (Figure7a) and hardly any
Pt backscatters are found in the ﬂ-EXAFS data of as-prepared Pt/SnO2 powders (Figure 7b). These
results are similar to recent data byin situEXAFS
on 3.0–12.0 wt% Pt-doped SnO2 prepared by
submicronic aerosol pyrolysis (Gaidi et al.,1998,
2000). However, no Pt-aggregates are found in our
Figure 6. Tin oxide crystal structure for platinum loadings of 0.0, 0.2 and 2.0 wt% (ﬂame 5/5). The highly crystalline cassiterite structure and the tin oxide crystallite size were not inﬂuenced by the addition of platinum. The small platinum loadings of 0.2 and 2.0 wt% cannot be detected (e.g. at about 46°).
Characterization of sensor made from platinum doped tin dioxide
Figure8 shows the response to small
concentra-tions of CO (5–50 ppm) of sensors which had been
in situ functionalized with 0.2 (on the left) and
2.0 wt% platinum (on the right). Doping the tin dioxide with 0.2 wt% platinum results in a much steeper calibration curve and the highest sensor signals compared to pure tin dioxide (see Fig-ure4). The higher sensor signal and especially the
higher sensitivity (i.e. the steeper response curve) increase sensor performance. Also in the case of platinum doping the best performance is achieved at a sensor operating temperature of 300°C.
However, the situation is completely diﬀerent when adding more platinum. Here, 2.0 wt% reduces the performance drastically and only at the highest concentration of 50 ppm the sensor starts to respond to CO. Note, that these tests were performed with a set of four sensors placed in a teﬂon-made chamber.
This is in agreement with the general ﬁndings on the inﬂuence of Pt-doping (i.e. functionalization) on the CO sensing properties of SnO2. The low
concentrations of platinum increases the signals to CO whereas increase in platinum concentration leads to the decrease in sensing properties. This was reported also for the sol-gel (or precipitated)
Table1. Surface composition determined from XPS-analysis and the binding energies of the diﬀerent peaks
Sample SnO2 0.2 wt% Pt–SnO2 2.0 wt% Pt–SnO2
Shift 6 eV for most of the sample No shifta No shift
C1s [at%] 22.7 41.3b 29.3b O1s [at%] 58.6 42.6 51.5 Sn3d5/2[at%] 18.6 16.0 19.0 Pt 4f [at%] – 0.02 0.1 Pt/Sn-ratioc – 0.0010:1 0.0058:1 O1s/eV 537.9 531.0 531.1 Pt 4f7/2/eV – 71.9 72.2 Pt 4f5/2/eV 75.5 75.4 Sn3d5/2/eV 487.1 (19.5%) 487.0 (57.1%) 487.1 493.9 (39.7) Sn3d3/2/eV 495.5 (12.9%) 495.4 (40.5%) 495.5 502.3 (27.8%) 502.3 (2.4%)d a
For a small fraction some shift was found (see at the Sn3d3/2peak). b
Note that the carbon stems from graphite below the sample (small sample size).
Determined by additional longer recording time of the Pt 4f and Sn 3d region.
dNote that this small fraction of Sn3d
3/2is due to partial charging of the sample which amounts to about 5%.
Figure 7. (a) XAS-spectra taken in the ﬂuorescence mode around the Pt L3-edge of 0.2 wt% Pt/SnO2and 2.0 wt% Pt/SnO2
SnO2 with 0.2 wt% (Pt/Sn ratio is 0.0016) and
2.0 wt% Pt (Pt/Sn ratio: 0.016). In this case the platinum was introduced either by impregnation of the pre-calcined SnO2with a platinum chloride
precursor or by precipitating it in solution before the thermal treatment (Kappler et al.,1998, 2001;
Cabot et al., 2000, 2001, 2002; Cabot, 2004).
Similar ﬁndings were reported for pyrosol co-deposited Pt/SnO2(Pt/Sn ratio: between 0.019 and
0.200) (Matko et al., 2002). In the wet phase
method the 0.2 wt% Pt doping increases signiﬁ-cantly the sensor signal to CO both in dry and especially in humid (50% r.h at 20°C) air, in contrast to 3.0 wt% Pt which decreases this property (Kappler, 2001). In both cases (for 0.2
and 2.0%) for the wet phase method Pt was found to be present in oxidized form (as Pt2+ or Pt4+)
and the formation of clusters or isolated metallic nanoparticles was not observed (Kappler, 1998,
2001; Cabot et al., 2000). In the aerosol pyrolysis
method Pt is found to be present as Pt clusters either in a metallic or in an oxidized state on the surface of SnO2 particles (Matko et al., 1999,
2002). In this case the best signals were observed
for a Pt/Sn ratio close to 0.019 (Matko et al., 1999).
The drastic eﬀect of the amount of platinum doping on sensing properties was investigated fur-ther at CO concentrations up to 1000 ppm (Fig-ure9, to eliminate consumption eﬀects these tests
were performed with one sensor in a chamber).
Also here doping with 0.2 wt% platinum results in the highest sensor signals compared to pure tin dioxide followed by the sensor with a doping of 2.0 wt%. However, the sensor with 2.0 wt%
Figure 8. Signal of SnO2sensors doped with 0.2 wt% Pt (left) and 2.0 wt% Pt (right) as a function of CO concentrations in
dry air at four temperatures. The signal increases with increasing CO concentration and decreasing sensor temperature. A power law dependence has been observed for all examined temperatures.
Figure 9. Sensor signal of diﬀerently doped sensors for diﬀerent CO concentrations in dry air and at 400°C. SnO2
with 0.2 wt% Pt (h, calibration function S=1+1.245C0.56) shows higher sensor signals than pure
SnO2 (s, calibration function S=1+0.918C0.49). SnO2
with 2.0 wt% Pt (n, calibration function S=1+0.038C0.88) shows the lowest sensor signals. This eﬀect becomes smaller with increasing CO concentration. The measurements were performed with one sensor in the chamber.
platinum is becoming more and more sensitive and the large diﬀerence in sensitivity becomes less at higher concentrations. The sensor signal can be approximated by a power law with respect to the CO concentration, i.e. S=1+aC b
Figure9 clearly indicates a diﬀerent behavior for
2.0 wt% platinum doping compared to pure tin oxide and 0.2 wt% Pt doping, respectively. This can be quantiﬁed by: the pre-factor (i.e. a in S=1+aCb
CO) of the power law ﬁt which is 0.918,
1.245, and 0.038 for 0.0, 0.2, and 2.0 wt%, respectively, and by the power law exponent (i.e. b in S=1+aCb
CO) of the power law ﬁt which is 0.49,
0.56, and 0.88 for 0.0, 0.2, and 2.0 wt%, respec-tively. The pre-factor is more than one order of magnitude diﬀerent for the 2.0 wt% platinum doping compared to the other sensors and the power law exponent also signiﬁcantly changes. The latter fact indicates a change in the type of reactive oxygen species involved in the reaction with CO (Barsan & Weimar,2001). At the operation
tem-perature more than one oxygen species can be present at the surface and their relative concen-tration could depend on the presence and amount of noble metal.
Although the eﬀect of the amount of platinum doping on SnO2 sensing properties is large, no
signiﬁcant diﬀerence in oxidation/chemical state of platinum on SnO2 has been observed for 0.2 and
2.0 wt% Pt, respectively. To summarize, only surface sensitive or element-speciﬁc methods such as XPS and EXAFS reveal information about the platinum functionalization. These methods revealed in both cases the presence of an oxidized form of platinum but show also a higher disper-sion in the case of 0.2 wt% Pt (smaller clusters). The absence of charging eﬀects for the platinum doped samples further indicates an embedding of the platinum within the tin dioxide lattice (see also the comparison of the resistance measurements in Figure11).
The detailed mechanism of CO detection by tin dioxide in the presence of platinum on its surface has not been clariﬁed yet. The eﬀect of platinum doping on sensor sensitivity is usually described by two mechanisms; the spill-over or catalytic eﬀect and Fermi energy control. In case of spill-over eﬀect, CO oxidation can be accelerated because of the activation, i.e. dissociation, of oxygen on platinum. Then the activated oxygen species reach the SnO2, where the ﬁnal reaction with CO takes
place. This results in shorter response time and larger sensitivity. This mechanism is generally accepted for Pt-doped SnO2gas sensors (Yamazoe,
1991). However, in the literature on catalytic
low-temperature CO oxidation on 0.2–2.0 wt% Pt-impregnated SnO2, a diﬀerent mechanism, i.e.
dissociative adsorption of oxygen on SnO2
fol-lowed by oxygen reverse spillover from the SnO2
onto Pt sites in isolated Pt-clusters and reaction with the CO chemisorbed on the Pt metal, is gen-erally accepted since the works of Boulahouache et al.(1992) and Grass and Lintz (1995, 1997a, b).
In this case (Fermi energy control) the electronic contact between SnO2and the noble metal particle
inﬂuences the electrical resistance (conductance) of the sensors (Matsushima et al., 1988; Yamazoe,
1991). At equilibrium, the Fermi level of the
cat-alyst and the semiconductor are at the same energy. The stoichiometry of the catalytically active noble metal particle/center (i.e. Pt or PtO2-X)
hereby depends on the composition of the ambient gas atmosphere and so does the position of its Fermi level. Consequently, the position of the Fermi level of SnO2and therefore the
concentra-tion of charge carriers (i.e. electrical resistance or conductance) will be inﬂuenced by surface reac-tions on the catalyst. This eﬀect, i.e. change in stoichiometry and chemical state of the platinum center (i.e. Pt or PtO2-X) on SnO2sensors, has been
recently observed and proved by in situ EXAFS
analysis (Gaidi et al.,1998, 2000).
The low signals to CO of the sensors with the high platinum loading (2.0 wt%) may result from ‘‘localized’’ CO consumption without electron transfer to the conduction band of SnO2. In this
case Pt acts as a ‘‘good catalyst’’ and catalytic oxidation of carbon monoxide takes place locally on platinum. In this case the charge transfer occurs only in a localized manner and has no direct impact on the electrical conduction of SnO2. In
order to validate this hypothesis, the analyte gas containing CO was introduced ﬁrst to an isolated sensor in a conﬁned measuring volume (position #1) and subsequently to a second measuring vol-ume where the sensors were arranged in sub-sequent directions of the ﬂow (position #2 to #5) with two sensors opposing each other (a, b). For this experiment 8 identical sensors were fabricated and simultaneously tested. Figure10 shows the
sensor response for 0.2 wt% platinum doping (left) and 2.0 wt% platinum doping (right). The
ﬁrst sensor (position #1) shows the highest signals followed by the sensors in the second chamber. In the second chamber a decrease of sensor signal at increasing downstream position is evident (Fig-ure10, left). All sensors with 0.2 wt% platinum
doping have a remarkable sensitivity for CO even at a reduced CO concentration because of its consumption at upstream sensors. Please note in comparison to previous data, that the consump-tion measurements were performed at 50% r.h. and therefore show slightly smaller signals towards CO. The situation is rather diﬀerent when increasing the platinum doping from 0.2 to 2.0 wt% (ﬁgure10, right). In this case only the
ﬁrst sensor is responding to CO, however, with much lower signals as for 0.2 wt% platinum doping. All other downstream sensors are almost not sensitive towards CO even at high CO con-centrations.
The drastic reduction in CO signal for ‘‘down-stream’’ sensors with high platinum loading (2.0 wt%) indicates higher CO consumption on them. It leads to the decrease in eﬀective CO concentration (which is seen by sensors), and therefore to the drastic decrease in the sensor sig-nals because of the non-linear sensor response (i.e. power law dependence on the CO concentration, e.g. see Figures4, 8 and 9). It should be noted that
higher platinum loadings resulted in low platinum dispersion (XPS, Table1) and usually, ﬂame-made
materials with higher Pt-content result in an easier reduction of platinum at higher loading (evidenced by EXAFS (Stark et al., 2005)). Therefore, the
‘‘localized’’ CO consumption without electron transfer to the conduction band of SnO2is likely.
However, this can be regarded only as a hypothesis and additional investigations are necessary. In general, a direct correlation between the sensing properties of Pt doped SnO2 with their catalytic
(i.e. ‘‘CO consumption’’) properties is desirable but rather diﬃcult. Recent studies also indicated that the inﬂuence of the substrate, heater (on the back side of the sensor substrate) and boundaries between oxide, Pt-electrodes and sensor substrate cannot be neglected making the situation even more complex (Kappler, 2001; Kappler et al.,
2001; Barsan & Weimar, 2003).
Stability of gas sensors
The sensors were tested for 20 days while every second day the sensors were exposed to three dif-ferent CO concentrations (i.e. to 10, 240 and 50 ppm) which were separated by 3 h. These tests were performed on two identical sensor pairs of pure SnO2 and doped with 0.2 wt% Pt placed
symmetrically into two chambers each. Figure11
shows the response of all four sensors. Identical sensors showed nearly identical resistance which indicates the high reproducibility. The platinum
Figure 10. Sensor signal of SnO2with 0.2 wt% Pt (left) and SnO2with 2.0 wt% Pt (right) for diﬀerent CO concentrations. In
both measurements, two test chambers are connected in series, the ﬁrst one containing a single sensor (#1) and the second one containing seven sensors (#2a to #5a). For 0.2 wt% Pt, the Sensor signal decreases subsequently in the direction of the gas ﬂow. For 2.0 wt% Pt, only the single sensor (#1) shows sensor signals, whereas all sensors in the second chamber show almost no sensor signals. The measurements have been performed at 450°C and in 50% relative humidity.
doped SnO2 sensors have lower resistance than
pure SnO2which might be beneﬁcial for the ﬁnal
device. These results are corroborated by the XPS analysis which showed a higher charging of the pure SnO2 sample. All sensors recover to their
initial resistance once the CO concentration is
back to zero. However, a small increase of the overall resistance at 0 ppm CO over time is observed. This small drift is less pronounced for the platinum doped sensor because of the surface stabilization eﬀect of platinum in the presence of CO. The stability of the platinum doped sensors is better than the undoped tin dioxide because the absorption/desorption equilibrium is reached fas-ter. This is further corroborated by the fact that essentially no drift has been observed at the pres-ence of CO (Figure12). The high stability of the
sensors derived from ﬂame-made powders becomes evident when comparing with sol-gel derived powders under the same conditions. This may be because of the high dispersion in the matrix and the well-crystalline nature of the ﬂame-made materials. The sol-gel-ﬂame-made powder drifts steadily over the entire time period which was evaluated (20 days) (Kappler,2001).
Summary and Conclusions
Gas sensors made from tin dioxide nanoparticles have been investigated for CO detection. Sensor characteristics were directly controlled by adjust-ing nanoparticle properties such as grain size and platinum functionalization. Here, ﬂame spray pyrolysis (FSP) was used to synthesize in one step SnO2 nanoparticles pure or Pt-doped with
con-trolled particle size and platinum content. Sensors made from SnO2 particles with a grain size of
10 nm show a 5 times higher sensor signal than particles of 20 nm and more than one order higher sensor signal than sensors made from 330 nm particles. The particle size control aﬀorded by FSP can be directly used to tune sensor perfor-mance without post-treatment of the sensing material. In situ functionalization (one-step) by
doping with platinum during FSP synthesis resulted in more sensitive sensors when containing 0.2 wt% Pt rather than 2.0 wt%. The latter showed a detrimental eﬀect because of the cata-lytic conversion of CO without electron transfer. CO consumption measurements and detailed structural analysis using XPS and EXAFS showed that Pt is incorporated as oxidized clusters. These oxidized platinum clusters were slightly reduced in vacuum during the XPS analysis. Furthermore, a low Pt concentration (0.2 wt%) seems to lead to a higher dispersion of Pt. The stability of the
Figure 11. Resistance of two identical pairs of SnO2sensors
(a) and (b) with 0.2 wt% Pt during exposure to three dif-ferent CO concentrations (10, 240 and 50 ppm) shown for the 4th day of a 20 days period. All sensors return to zero setting upon end of the exposure showing excellent repro-ducibility and stability.
Figure 12. Resistance of SnO2/0.2 wt% Pt sensors over
20 days in air and in 10, 50 and 240 ppm CO. The mea-surement was performed at 400°C and in 10% relative humidity. Excellent reproducibility and stability is observed over that period and CO concentration.
sensors was tested and found suitable for low level CO detection: <10 ppm according to European legislation and 50 according to US.
We would like to thank Dr. Frank Krumeich for providing the HRTEM, STEM and EDX analyses and Dr. Stefan Mangold for assistance in using beam line ANKA-XAS and the ﬂuorescence detection at the Synchrotron Radiation Facility ANKA of Forschungszentrum Karlsruhe. The EXAFS studies were supported within the project XAS_03_030 by the European Community-Research Infrastructure Action under the FP6: ‘‘Structuring the European Research Area’’. (Integrating Activity on Synchrotron and Free Electron Laser Science (IA-SFS) RII3-CT-2004-506008).
Barsan N., M. Schweizer-Berberich & W. Gopel, 1999. Fun-damental and practical aspects in the design of nanoscaled SnO2 gas sensors: a status report. Fres. J. Anal. Chem. 365(4), 287–304.
Barsan N. & U. Weimar, 2001. Conduction model of metal oxide gas sensors. J. Electroceram. 7(3), 143–167.
Barsan N. & U. Weimar, 2003. Understanding the fundamen-tal principles of mefundamen-tal oxide based gas sensors; the example of CO sensing with SnO2sensors in the presence of humidity. J. Phys. Cond. Matter 15(20), R813–R839.
Bazin D., H. Dexpert, J. Lynch & J.P. Bournonville, 1999. XAS of electronic state correlations during the reduction of the bimetallic PtRe/Al2O3system. J. Synchr. Rad. 7, 465. Bolzan A.A., C. Fong, B.J. Kennedy & C.J. Howard, 1997.
Structural studies of rutile-type metal dioxides. Acta Crystall. Section B – Struct. Sci. 53(3), 373–380.
Boulahouache A., G. Kons, H.G. Lintz & P. Schulz, 1992. Oxidation of carbon-monoxide on platinum tin dioxide catalysts at low-temperatures. Appl. Catal. – Gen. 91(2), 115–123.
Cabot A., 2004. Inﬂuence of Catalytic Additives on Metal Oxide Nanoparticles for Gas Sensing Applications. Barce-lona: Universitat de Barcelona.
Cabot A., J. Arbiol, J.R. Morante, U. Weimar, N. Barsan & W. Gopel, 2000. Analysis of the noble metal catalytic additives introduced by impregnation of as obtained SnO2 sol-gel nanocrystals for gas sensors. Sensors Actuators B – Chemical 70(1–3), 87–100.
Cabot A., A. Dieguez, A. Romano-Rodriguez, J.R. Morante & N. Barsan, 2001. Inﬂuence of the catalytic introduction procedure on the nano- SnO2 gas sensor performances – where and how stay the catalytic atoms?. Sensors Actuators B – Chemical 79(2–3), 98–106.
Cabot A., A. Vila & J.R. Morante, 2002. Analysis of the catalytic activity and electrical characteristics of diﬀerent modiﬁed SnO2layers for gas sensors. Sensors Actuators B – Chemical 84(1), 12–20.
Cheary R.W. & A.A. Coelho, 1998. Axial divergence in a conventional X-ray powder diﬀractometer. I. Theoretical foundations. J. Appl. Crystallogr. 31, 851–861.
Dieguez A., A. Vila, A. Cabot, A. Romano-Rodriguez, J.R. Morante, J. Kappler, N. Barsan, U. Weimar & W. Gopel, 2000. Inﬂuence on the gas sensor performances of the metal chemical states introduced by impregnation of calcinated SnO2sol-gel nanocrystals. Sensors Actuators B – Chemical 68(1–3), 94–99.
EN. 2000. Directive 2000/69/EC of the European parliament and of the council. Oﬃcial Journal of the European Commission, L313/12.
Eranna G., B.C. Joshi, D.P. Runthala & R.P. Gupta, 2004. Oxide materials for development of integrated gas sensors – a comprehensive review. Crit. Rev. Solid State Mat. Sci. 29(3– 4), 111–188.
Gaidi M., J.L. Hazemann, I. Matko, B. Chenevier, M. Rumyantseva, A. Gaskov & M. Labeau, 2000. Role of Pt aggregates in Pt/SnO2 thin ﬁlms used as gas sensors – investigations of the catalytic eﬀect. J. Electrochem. Soc. 147(8), 3131–3138.
Gaidi M., M. Labeau, B. Chenevier & J.L. Hazemann, 1998. In-situ EXAFS analysis of the local environment of Pt particles incorporated in thin ﬁlms of SnO2 semi-conductor oxide used as gas-sensors. Sensors Actuators B – Chemical 48(1–3), 277–284.
Grandjean D., R.E. Benﬁeld, C. Nayral, A. Maisonnat & B. Chaudret, 2004. EXAFS and XANES Study of a Pure and Pd Doped Novel Sn/SnOxnanomaterial. J. Phys. Chem. B 108(26), 8876–8887.
Grass K. & H.G. Lintz, 1995. Tin(IV)oxide supported noble metal catalysts for the carbon monoxide oxidation at low temperatures. Preparation of Catalysts VI: Studies in surface science and catalysis, Elsevier Science Publ., Amsterdam, pp. 1111–1119.
Grass K. & H.G. Lintz, 1997a. The kinetics of carbon monoxide oxidation on tin(IV) oxide supported platinum catalysts. J. Catal. 172(2), 446–452.
Grass K. & H.G. Lintz, 1997b. Oxidation of carbon monoxide over platinum–tin(IV) oxide catalysts: an example of spill-over catalysis?. Spillspill-over Migration Surface Species on Catalysts 112, 135–142.
Grunwaldt J.D., U. Gobel & A. Baiker, 1997. Preparation and characterization of thin TiO2-ﬁlms on gold/mica. Fres. J. Anal. Chem. 358(1–2), 96–100.
Iwasawa Y. 1996. Characterization and Chemical Design of Oxide Surfaces. 11th International Congress on Catalysis, Baltimore, pp. 21–34.
Johannessen T. & S. Koutsopoulos, 2002. One-step ﬂame synthesis of an active Pt/TiO2catalyst for SO2oxidation – a possible alternative to traditional methods for parallel screening. J. Catal. 205(2), 404–408.
Kappen P., L. Tro¨ger, G. Materlik, C. Reckleben, K. Hansen, J.-D. Grunwaldt & B.S. Clausen, 2002. Silicon drift detectors as a tool for time-resolved ﬂuorescence XAFS on low-concentrated samples in catalysis. J. Sync. Rad. 9, 246–253. Kappler J., 2001. Characterization of high-performance SnO2 gas sensors for CO detection by in situ techniques. Aachen: Saker Verlag.
Kappler J., N. Barsan, U. Weimar, A. Dieguez, J.L. Alay, A. Romano-Rodriguez, J.R. Morante & W. Gopel, 1998. Correlation between XPS, Raman and TEM measurements and the gas sensitivity of Pt and Pd doped SnO2based gas sensors. Fres. J. Anal. Chem. 361(2), 110–114.
Kappler J., A. Tomescu, N. Barsan & U. Weimar, 2001. CO consumption of Pd doped SnO2based sensors. Thin Solid Films 391(2), 186–191.
Kim K.S., N. Winograd & R.E. Davis, 1971. Electron spectroscopy of platinum-oxygen surfaces and application to electrochemical studies. J. Am. Chem. Soc. 93(23), 6296– 6297.
Ma¨dler L., H.K. Kammler, R. Mueller & S.E. Pratsinis, 2002a. Controlled synthesis of nanostructured particles by ﬂame spray pyrolysis. J. Aerosol Sci. 33(2), 369–389.
Ma¨dler L. & S.E. Pratsinis, 2002. Bismuth oxide nanoparticles by ﬂame spray pyrolysis. J. Am. Ceramic Soc. 85(7), 1713– 1718.
Ma¨dler L., W.J. Stark & S.E. Pratsinis, 2002b. Flame-made ceria nanoparticles. J. Mater. Res. 17(6), 1356–1362. Ma¨dler L., W.J. Stark & S.E. Pratsinis, 2003. Simultaneous
deposition of Au nanoparticles during ﬂame synthesis of TiO2and SiO2. J. Mater. Res. 18(1), 115–120.
Matko I., M. Gaidi, B. Chenevier, A. Charai, W. Saikaly & M. Labeau, 2002. Pt doping of SnO2thin ﬁlms – a transmission electron microscopy analysis of the porosity evolution. J. Electrochem. Soc. 149(8), H153–H158.
Matko I., M. Gaidi, J.L. Hazemann, B. Chenevier & M. Labeau, 1999. Electrical properties under polluting gas (CO) of Pt- and Pd-doped polycrystalline SnO2thin ﬁlms: analysis of the metal aggregate size eﬀect. Sensors Actuators B – Chemical 59(2–3), 210–215.
Matsushima S., Y. Teraoka, N. Miura & N. Yamazoe, 1988. Electronic interaction between metal additives and tin dioxide in tin dioxide-based gas sensors. Jap. J. Appl. Phys., Part 1: Regular Papers, Short Notes & Review Papers 27(10), 1798–1802.
Muilenberg G.E., 1979. Handbook of Photoelectron Spectros-copy. Eden Prairie, Minnesota: Perkin-Elmer Corp. Pearce T.C., S.S. Schiﬀman, H.T. Nagle & J.W. Gardner,. 2004.
Handbook of Machine Olfaction: Electronic Nose Technol-ogy. Weinheim: Wiley-VCH Verlag GmbH.
Ressler T., 1998. WinXAS: a program for X-ray absorption spectroscopy data analysis under MS-Windows. J. Synchr. Rad. 5, 118.
Rothschild A. & Y. Komem, 2004. The eﬀect of grain size on the sensitivity of nanocrystalline metal-oxide gas sensors. J. Appl. Phys. 95(11), 6374–6380.
Sahm T., A. Gurlo, N. Barsan & U. Weimar, Properties of indium oxide semiconducting sensors deposited by diﬀerent techniques. J. Particulate Sci. (submitted).
Sahm T., A. Gurlo, N. Baˆrsan, U. Weimar & L. Ma¨dler, 2005. Fundamental studies on SnO2by means of simultaneous work function change and conduction measurements. Thin Solid Films 490(1), 43–47.
Sahm T., L. Ma¨dler, A. Gurlo, N. Barsan, S.E. Pratsinis & U. Weimar, 2004. Flame spray synthesis of tin dioxide nano-particles for gas sensing. Sensors Actuators B – Chemical 98(2–3), 148–153.
Schweizer-Berberich M., J.G. Zheng, U. Weimar, W. Gopel, N. Barsan, E. Pentia & A. Tomescu, 1996. The eﬀect of Pt and Pd surface doping on the response of nanocrystalline tin dioxide gas sensors to CO. Sensors Actuators B – Chemical 31(1–2), 71–75.
Stark W.J., J.-D. Grunwaldt, M. Maciejewski, S.E. Pratsinis & A. Baiker, 2005. Improved thermal stability of ﬂame-made pt/ceria/zirconia for low-temperature oxygen exchange. Chem. Mat. 17, 3352–3359.
Strobel R., W.J. Stark, L. Ma¨dler, S.E. Pratsinis & A. Baiker, 2003. Flame-made platinum/alumina: structural properties and catalytic behaviour in enantioselective hydrogenation. J. Catal. 213(2), 296–304.
Tani T., L. Ma¨dler & S.E. Pratsinis, 2002. Homogeneous ZnO nanoparticles by ﬂame spray pyrolysis. J. Nanoparticle Res. 4(4), 337–343.
Xu C., J. Tamaki, N. Miura & N. Yamazoe, 1991. Grain-size eﬀects on gas sensitivity of porous SnO2-based elements. Sensors Actuators B – Chemical 3(2), 147–155.
Yamazoe N., 1991. New approaches for improving semicon-ductor gas sensors. Sensors Actuators, B: Chemical B 5(1–4), 7–19.
Yang J.C., Y.C. Kim, Y.G. Shul, C.H. Shin & T.K. Lee, 1997. Characterization of photoreduced Pt/TiO2 and decomposi-tion of dichloroacetic acid over photoreduced Pt/TiO2 catalysts. Appl. Surf. Sci. 121, 525–529.